The effect of the disposition of coordinated oxygen atoms on the magnitude of the energy barrier for magnetization reversal in a family of linear trinuclear Zn-Dy-Zn complexes with a square-antiprism DyO8 coordination sphere.
Oyarzabal, Itziar; Rodríguez-Diéguez, Antonio; Barquín, Montserrat; Seco, José M; Colacio, Enrique; Dalton transactions (Cambridge, England : 2003) 46 (2017) 4278–4286; doi:10.1039/c7dt00138j

data_7042290
_publ_section_title
;
 The effect of the disposition of coordinated oxygen atoms on the
 magnitude of the energy barrier for magnetization reversal in a family of
 linear trinuclear Zn-Dy-Zn complexes with a square-antiprism DyO8
 coordination sphere.
;
_journal_issue                   13
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              4278
_journal_page_last               4286
_journal_paper_doi               10.1039/c7dt00138j
_journal_volume                  46
_journal_year                    2017
_chemical_formula_sum            'C43 H52 Br6 Dy N5 O14 Zn2'
_chemical_formula_weight         1635.59
_chemical_name_systematic
;
 ?
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014
_audit_update_record
;
2016-12-22 deposited with the CCDC.
2017-02-28 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 115.170(3)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   14.6274(3)
_cell_length_b                   27.3664(5)
_cell_length_c                   14.7306(4)
_cell_measurement_reflns_used    7764
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      27.7960
_cell_measurement_theta_min      1.7900
_cell_volume                     5336.8(2)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.28 (release 01-02-2013 CrysAlis171 .NET)
(compiled Feb  1 2013,16:14:44)
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.28 (release 01-02-2013 CrysAlis171 .NET)
(compiled Feb  1 2013,16:14:44)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.28 (release 01-02-2013 CrysAlis171 .NET)
(compiled Feb  1 2013,16:14:44)
;
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.893
_diffrn_measurement_device_type  'SuperNova, Single source at offset, Eos'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0564
_diffrn_reflns_av_unetI/netI     0.0819
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.893
_diffrn_reflns_limit_h_max       19
_diffrn_reflns_limit_h_min       -18
_diffrn_reflns_limit_k_max       27
_diffrn_reflns_limit_k_min       -35
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            25751
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.893
_diffrn_reflns_theta_full        25.000
_diffrn_reflns_theta_max         28.284
_diffrn_reflns_theta_min         1.538
_diffrn_source                   'SuperNova (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    6.836
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.46060
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.28 (release 01-02-2013 CrysAlis171 .NET)
(compiled Feb  1 2013,16:14:44)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    2.036
_exptl_crystal_description       prismatic
_exptl_crystal_F_000             3172
_exptl_crystal_size_max          0.28
_exptl_crystal_size_mid          0.14
_exptl_crystal_size_min          0.12
_refine_diff_density_max         2.139
_refine_diff_density_min         -2.347
_refine_diff_density_rms         0.199
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.026
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     650
_refine_ls_number_reflns         11840
_refine_ls_number_restraints     28
_refine_ls_restrained_S_all      1.036
_refine_ls_R_factor_all          0.0811
_refine_ls_R_factor_gt           0.0533
_refine_ls_shift/su_max          0.026
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0387P)^2^+26.9790P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1085
_refine_ls_wR_factor_ref         0.1235
_reflns_Friedel_coverage         0.000
_reflns_number_gt                8854
_reflns_number_total             11840
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c7dt00138j2.cif
_cod_data_source_block           Compound3
_cod_depositor_comments
'Adding full bibliography for 7042287--7042292.cif.'
_cod_database_code               7042290
_shelxl_version_number           2014-3
_shelx_res_checksum              5733